Modelling and Simulation in Engineering
Volume 2016 (2016), Article ID 5934814, 5 pages
http://dx.doi.org/10.1155/2016/5934814

Research Article

A Note on Torsion of Nonlocal Composite Nanobeams

Luciano Feo and Rosa Penna

Department of Civil Engineering, University of Salerno, Via Ponte don Melillo, 84084 Fisciano, Italy

Received 4 December 2015; Accepted 5 October 2016

Academic Editor: Theodoros C. Rousakis

Copyright © 2016 Luciano Feo and Rosa Penna. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

The ERINGEN elastic constitutive relation is used in this paper in order to assess small-scale effects in nanobeams. Structural behavior is studied for functionally graded materials in the cross-sectional plane and torsional loading conditions. The governing boundary value problem has been formulated in a mixed framework. Torsional rotations and equilibrated moments are evaluated by solving a first-order differential equation of elastic equilibrium with boundary conditions of kinematic-type. Benchmarks examples are briefly discussed, enlightening thus effectiveness of the proposed methodology.

1. Introduction

Assessments of stress and displacement fields in continuous media are a subject of special interest in the theory of structures. Numerous case studies have been examined in the current literature with reference to beams [1–6], half-spaces [7, 8], thin plates [9, 10], compressible cubes [11], and concrete [12, 13]. Several methodologies of analysis have been developed in the research field of geometric continuum mechanics [14, 15], limit analysis [16–19], homogenization [20], elastodynamics [21–25], thermal problems [26–28], random composites [29–32], and nonlocal and gradient formulations [33–38]. A comprehensive analysis of classical and generalized models of elastic structures, with special emphasis on rods, can be found in the interesting book by I [39]. In particular, I [40–42] formulated a method for the solution of SAINT-VENANT problems in micropolar beams with arbitrary cross-section. Detailed solution of the torsion problem for an isotropic micropolar beam with circular cross-section is given in [43, 44]. Experimental investigations are required for the evaluation of the behavior of composite structures [45].

In the context of the present research, particular attention is devoted to the investigation of scale effects in nanostructures; see, for example, [46–55] and the reviews [56, 57]. Recent contributions on functionally graded materials have been developed for nanobeams under flexure [58, 59] and torsion [60].

Unlike previous treatments on torsion of gradient elastic bars (see, e.g., [61]) in which higher-order boundary conditions have to be enforced, this paper is concerned with the analysis of composite nanobeams with nonlocal constitutive behavior conceived by ERINGEN in [62]. Basic equations governing the ERINGEN model are preliminarily recalled in Section 2. The corresponding elastic equilibrium problem of torsion of an ERINGEN circular nanobeam is then formulated in Section 3. It is worth noting that only classical boundary conditions are involved in the present study. Small-scale effects are detected in Section 4 for two static schemes of applicative interest. Some concluding remarks are delineated in Section 5.

2. Eringen Nonlocal Elastic Model

Before formulating the elastostatic problem of a nonlocal nanobeam subjected to torsion, we shortly recall in the sequel some notions of nonlocal elasticity. To this end, let us consider a body made of a material, possibly composite, characterized by the following integral relation between the stress at a point and the elastic strain field in [62]:

The fourth-order tensor , symmetric and positive definite, describes the material elastic stiffness at the point .

The attenuation function depends on the Euclidean distance and on a nonlocal dimensionless parameter defined by

where is a material constant, is an internal characteristic length, and stands for external characteristic length.

Assuming a suitable expression of the nonlocal modulus in terms of a variant of the BESSEL function, we get the inverse differential relationship of (1) between the nonlocal stress and the elastic deformation

with the Laplacian. Note that (3) can be conveniently used in order to describe the law between the nonlocal shear stress field on the cross-section of a nanobeam and the elastic shear strain as follows:

where is the axial direction and is the shear modulus.

3. Torsion of Nonlocal Circular Nanobeams

Let be the cross-section of a circular nanobeam, of length , subjected to the following loading conditions depicted in Figure 1:

The triplet describes a set of Cartesian axes originating at the left cross-section centre

Figure 1: Sketch of a nanobeam under torsion.

Equilibrium equations are expressed by

where is the twisting moment.

Components of the displacement field, up to a rigid body motion, of a circular nanobeam under torsion write as

where is the torsional rotation of the cross-section at the abscissa . Shear strains, compatible with the displacement field equation (7), are given by

where

is the twisting curvature. The shear modulus is assumed to be functionally graded only in the cross-sectional plane .

The elastic twisting stiffness is provided by

where the symbol is the inner product between vectors.

The differential equation of nonlocal elastic equilibrium of a nanobeam under torsion is formulated as follows. Let us preliminarily multiply (4) by and integrate on

with the vector given by (8).

Enforcing (6a) and imposing the static equivalence condition

we get the relation

This equation can be interpreted as decomposition formula of the twisting curvature into elastic and inelastic parts

with

Accordingly, the scale effect exhibited by the torsional rotation function of a nonlocal nanobeam can be evaluated by solving a corresponding linearly elastic beam subjected to the twisting curvature distortion (15b).

4. Benchmark Examples

Let us consider a nanocantilever and a fully clamped nanobeam of length subjected to the following quadratic distribution of couples per unit length:

The cross-sectional torsional rotation is evaluated by following the methodology illustrated in the previous section. The nonlocality effect is assessed by prescribing the twisting curvature distortion equation (15b)

on corresponding (cantilever and fully clamped) local nanobeams. Let us set and . Torsional rotations versus of both the nanobeams are displayed in Figures 2 and 3 for selected values of the nonlocal parameter .

Figure 2: Torsional rotation for the nanocantilever versus for increasing values of .

Figure 3: Dimensionless torsional rotation for the fully clamped nanobeam versus for increasing values of .

5. Concluding Remarks

The basic outcomes contributed in the present paper are listed as follows:

(1)Size-effects in nanobeams under torsion have been evaluated by resorting to the nonlocal theory of elasticity.(2)Exact torsional rotations solutions of cross-sections of functionally graded nanobeams have been established for nanocantilevers and fully clamped nanobeams under a quadratic distribution of couples per unit length.(3)It has been observed that the stiffness of a nanobeam under torsional loadings is affected by the scale parameter and depends on the boundary kinematic constraints. Indeed, as shown in Figures 2 and 3, contrary to the nanocantilever structural behavior, the fully clamped nanobeam becomes stiffer for increasing values of the nonlocal parameter.

Competing Interests

There is no conflict of interests related to this paper.

References

R. Barretta, “On Cesàro-Volterra method in orthotropic Saint-Venant beam,” Journal of Elasticity, vol. 112, no. 2, pp. 233–253, 2013.

R. Barretta and M. Diaco, “On the shear centre in Saint-Venant beam theory,” Mechanics Research Communications, vol. 52, pp. 52–56, 2013.

G. Romano, A. Barretta, and R. Barretta, “On torsion and shear of Saint-Venant beams,” European Journal of Mechanics. A. Solids, vol. 35, pp. 47–60, 2012.

R. Barretta, “On stress function in Saint-Venant beams,” Meccanica, vol. 48, no. 7, pp. 1811–1816, 2013.

F. Marmo and L. Rosati, “Analytical integration of elasto-plastic uniaxial constitutive laws over arbitrary sections,” International Journal for Numerical Methods in Engineering, vol. 91, no. 9, pp. 990–1022, 2012.

F. Marmo and L. Rosati, “The fiber-free approach in the evaluation of the tangent stiffness matrix for elastoplastic uniaxial constitutive laws,” International Journal for Numerical Methods in Engineering, vol. 94, no. 9, pp. 868–894, 2013.

L. Rosati and F. Marmo, “Closed-form expressions of the thermo-mechanical fields induced by a uniform heat source acting over an isotropic half-space,” International Journal of Heat and Mass Transfer, vol. 75, pp. 272–283, 2014.

F. Marmo and L. Rosati, “A general approach to the solution of Boussinesq's problem for polynomial pressures acting over polygonal domains,” Journal of Elasticity, vol. 122, no. 1, pp. 75–112, 2016.

R. Barretta, “Analogies between Kirchhoff plates and Saint-Venant beams under torsion,” Acta Mechanica, vol. 224, no. 12, pp. 2955–2964, 2013.

R. Barretta, “Analogies between Kirchhoff plates and Saint-Venant beams under flexure,” Acta Mechanica, vol. 225, no. 7, pp. 2075–2083, 2014.

A. M. Tarantino, “Homogeneous equilibrium configurations of a hyperelastic compressible cube under equitriaxial dead-load tractions,” Journal of Elasticity, vol. 92, no. 3, pp. 227–254, 2008.

V. A. Salomoni, G. Mazzucco, C. Pellegrino, and C. E. Majorana, “Three-dimensional modelling of bond behaviour between concrete and FRP reinforcement,” Engineering Computations, vol. 28, no. 1, pp. 5–29, 2011.

V. A. Salomoni, C. E. Majorana, B. Pomaro, G. Xotta, and F. Gramegna, “Macroscale and mesoscale analysis of concrete as a multiphase material for biological shields against nuclear radiation,” International Journal for Numerical and Analytical Methods in Geomechanics, vol. 38, no. 5, pp. 518–535, 2014.

G. Romano, R. Barretta, and M. Diaco, “The geometry of nonlinear elasticity,” Acta Mechanica, vol. 225, no. 11, pp. 3199–3235, 2014.

G. Romano, R. Barretta, and M. Diaco, “Geometric continuum mechanics,” Meccanica, vol. 49, no. 1, pp. 111–133, 2014.

A. Caporale, R. Luciano, and L. Rosati, “Limit analysis of masonry arches with externally bonded FRP reinforcements,” Computer Methods in Applied Mechanics and Engineering, vol. 196, no. 1–3, pp. 247–260, 2006.

A. Caporale and R. Luciano, “Limit analysis of masonry arches with finite compressive strength and externally bonded reinforcement,” Composites Part B: Engineering, vol. 43, no. 8, pp. 3131–3145, 2012.

A. Caporale, L. Feo, R. Luciano, and R. Penna, “Numerical collapse load of multi-span masonry arch structures with FRP reinforcement,” Composites Part B: Engineering, vol. 54, no. 1, pp. 71–84, 2013.

A. Caporale, L. Feo, D. Hui, and R. Luciano, “Debonding of FRP in multi-span masonry arch structures via limit analysis,” Composite Structures, vol. 108, no. 1, pp. 856–865, 2014.

F. Greco and R. Luciano, “A theoretical and numerical stability analysis for composite micro-structures by using homogenization theory,” Composites Part B: Engineering, vol. 42, no. 3, pp. 382–401, 2011.

A. M. Tarantino, “Nonlinear fracture mechanics for an elastic Bell material,” The Quarterly Journal of Mechanics and Applied Mathematics, vol. 50, no. 3, pp. 435–456, 1997.

A. M. Tarantino, “The singular equilibrium field at the notch-tip of a compressible material in finite elastostatics,” Journal of Applied Mathematics and Physics, vol. 48, no. 3, pp. 370–388, 1997.

A. M. Tarantino, “On extreme thinning at the notch tip of a neo-Hookean sheet,” The Quarterly Journal of Mechanics and Applied Mathematics, vol. 51, no. 2, pp. 179–190, 1998.

A. M. Tarantino, “On the finite motions generated by a mode I propagating crack,” Journal of Elasticity, vol. 57, no. 2, pp. 85–103, 1999.

A. M. Tarantino, “Crack propagation in finite elastodynamics,” Mathematics and Mechanics of Solids, vol. 10, no. 6, pp. 577–601, 2005.

V. A. Salomoni, C. E. Majorana, G. M. Giannuzzi, and A. Miliozzi, “Thermal-fluid flow within innovative heat storage concrete systems for solar power plants,” International Journal of Numerical Methods for Heat and Fluid Flow, vol. 18, no. 7-8, pp. 969–999, 2008.

F. Marotti de Sciarra and M. Salerno, “On thermodynamic functions in thermoelasticity without energy dissipation,” European Journal of Mechanics. A. Solids, vol. 46, pp. 84–95, 2014.

G. Xotta, G. Mazzucco, V. A. Salomoni, C. E. Majorana, and K. J. Willam, “Composite behavior of concrete materials under high temperatures,” International Journal of Solids and Structures, vol. 64, pp. 86–99, 2015.

R. Luciano and J. R. Willis, “Bounds on non-local effective relations for random composites loaded by configuration-dependent body force,” Journal of the Mechanics and Physics of Solids, vol. 48, no. 9, pp. 1827–1849, 2000.

R. Luciano and J. R. Willis, “Non-local effective relations for fibre-reinforced composites loaded by configuration-dependent body forces,” Journal of the Mechanics and Physics of Solids, vol. 49, no. 11, pp. 2705–2717, 2001.

R. Luciano and J. R. Willis, “Boundary-layer corrections for stress and strain fields in randomly heterogeneous materials,” Journal of the Mechanics and Physics of Solids, vol. 51, no. 6, pp. 1075–1088, 2003.

R. Luciano and J. R. Willis, “Hashin-Shtrikman based FE analysis of the elastic behaviour of finite random composite bodies,” International Journal of Fracture, vol. 137, no. 1–4, pp. 261–273, 2006.

R. De Borst and H.-B. Muehlhaus, “Gradient-dependent plasticity: formulation and algorithmic aspects,” International Journal for Numerical Methods in Engineering, vol. 35, no. 3, pp. 521–539, 1992.

E. C. Aifantis, “Strain gradient interpretation of size effects,” International Journal of Fracture, vol. 95, no. 1–4, pp. 299–314, 1999.

E. C. Aifantis, “Gradient deformation models at nano, micro, and macro scales,” Journal of Engineering Materials and Technology, Transactions of the ASME, vol. 121, no. 2, pp. 189–202, 1999.

R. H. J. Peerlings, R. De Borst, W. A. M. Brekelmans, and J. H. P. De Vree, “Gradient enhanced damage for quasi-brittle materials,” International Journal for Numerical Methods in Engineering, vol. 39, no. 19, pp. 3391–3403, 1996.

R. H. J. Peerlings, M. G. D. Geers, R. de Borst, and W. A. M. Brekelmans, “A critical comparison of nonlocal and gradient-enhanced softening continua,” International Journal of Solids and Structures, vol. 38, no. 44-45, pp. 7723–7746, 2001.

H. Askes and E. C. Aifantis, “Gradient elasticity in statics and dynamics: an overview of formulations, length scale identification procedures, finite element implementations and new results,” International Journal of Solids and Structures, vol. 48, no. 13, pp. 1962–1990, 2011.

D. Ieşan, “Classical and generalized models of elastic rods,” in Modern Mechanics and Mathematics, D. Gao and R. W. Ogden, Eds., CRC Series, CRC Press, 2008.

D. Ieşan, “Saint-Venant's problem in micropolar elasticity,” in Mechanics of Micropolar Media, O. Brulin and R. K. T. Hsieh, Eds., pp. 281–390, World Scientific, Singapore, 1982.

D. Ieşan, “Generalized twist for the torsion of micropolar cylinders,” Meccanica, vol. 21, no. 2, pp. 94–96, 1986.

D. Ieşan, “Generalized torsion of elastic cylinders with microstructure,” Note di Matematica, vol. 27, no. 2, pp. 121–130, 2007.

R. D. Gauthier and W. E. Jahsman, “Quest for micropolar elastic constants,” Journal of Applied Mechanics, Transactions ASME, vol. 42, no. 2, pp. 369–374, 1975.

G. V. K. Reddy and N. K. Venkatasubramanian, “Saint-Venant's problem for a micropolar elastic circular cylinder,” International Journal of Engineering Science, vol. 14, no. 11, pp. 1047–1057, 1976.

G. Dinelli, G. Belz, C. E. Majorana, and B. A. Schrefler, “Experimental investigation on the use of fly ash for lightweight precast structural elements,” Materials and Structures/Materiaux et Constructions, vol. 29, no. 194, pp. 632–638, 1996.

J. Peddieson, G. R. Buchanan, and R. P. McNitt, “Application of nonlocal continuum models to nanotechnology,” International Journal of Engineering Science, vol. 41, no. 3–5, pp. 305–312, 2003.

J. N. Reddy, “Nonlocal theories for bending, buckling and vibration of beams,” International Journal of Engineering Science, vol. 45, no. 2–8, pp. 288–307, 2007.

Q. Wang and K. M. Liew, “Application of nonlocal continuum mechanics to static analysis of micro- and nano-structures,” Physics Letters, Section A: General, Atomic and Solid State Physics, vol. 363, no. 3, pp. 236–242, 2007.

M. Aydogdu, “A general nonlocal beam theory: its application to nanobeam bending, buckling and vibration,” Physica E: Low-Dimensional Systems and Nanostructures, vol. 41, no. 9, pp. 1651–1655, 2009.

O. Civalek and Ç. Demir, “Bending analysis of microtubules using nonlocal Euler-Bernoulli beam theory,” Applied Mathematical Modelling, vol. 35, no. 5, pp. 2053–2067, 2011.

H.-T. Thai and T. P. Vo, “A nonlocal sinusoidal shear deformation beam theory with application to bending, buckling, and vibration of nanobeams,” International Journal of Engineering Science, vol. 54, pp. 58–66, 2012.

R. Barretta and F. Marotti De Sciarra, “A nonlocal model for carbon nanotubes under axial loads,” Advances in Materials Science and Engineering, vol. 2013, Article ID 360935, 6 pages, 2013.

F. Marotti de Sciarra and R. Barretta, “A gradient model for Timoshenko nanobeams,” Physica E: Low-Dimensional Systems and Nanostructures, vol. 62, pp. 1–9, 2014.

R. Barretta, L. Feo, R. Luciano, and F. Marotti de Sciarra, “Application of an enhanced version of the Eringen differential model to nanotechnology,” Composites B, vol. 96, pp. 274–280, 2016.

R. Barretta, L. Feo, R. Luciano, F. Marotti de Sciarra, and R. Penna, “Functionally graded Timoshenko nanobeams: a novel nonlocal gradient formulation,” Composites B, vol. 100, pp. 208–219, 2016.

B. Arash and Q. Wang, “A review on the application of nonlocal elastic models in modeling of carbon nanotubes and graphenes,” Computational Materials Science, vol. 51, no. 1, pp. 303–313, 2012.

R. Rafiee and R. M. Moghadam, “On the modeling of carbon nanotubes: a critical review,” Composites Part B: Engineering, vol. 56, pp. 435–449, 2014.

R. Barretta, R. Luciano, and F. M. de Sciarra, “A fully gradient model for Euler-Bernoulli nanobeams,” Mathematical Problems in Engineering, vol. 2015, Article ID 495095, 8 pages, 2015.

M. A. Eltaher, S. A. Emam, and F. F. Mahmoud, “Static and stability analysis of nonlocal functionally graded nanobeams,” Composite Structures, vol. 96, pp. 82–88, 2013.

F. Marotti de Sciarra, M. Čanadija, and R. Barretta, “A gradient model for torsion of nanobeams,” Comptes Rendus—Mecanique, vol. 343, no. 4, pp. 289–300, 2015.

K. A. Lazopoulos and A. K. Lazopoulos, “On the torsion problem of strain gradient elastic bars,” Mechanics Research Communications, vol. 45, pp. 42–47, 2012.

A. C. Eringen, “On differential equations of nonlocal elasticity and solutions of screw dislocation and surface waves,” Journal of Applied Physics, vol. 54, no. 9, pp. 4703–4710, 1983.